1.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, Nov-Dec. 2012 pp-4547-4558 ISSN: 2249-6645 An Overview of Clearance Optimization in Sheet Metal Blanking Process Prof. T. Z. Quazi, 1 R.S.Shaikh2 1, 2 Department of Mechanical Engineering, Mumbai University, IndiaAbstract: This document prescribes a model investigation the effect of potential parameters influencing the blankingprocess and their interaction. The blanking process optimization carried out by using Design of Experiment (DOE), FiniteElement Method (FEM) with ANSYS Package, Simulation with ABAQUS-Explicit software, Blank soft Software and NeuralNetwork Simulation in order to achieve the intended model objectives.Keywords: Blanking Process, DOE, FEM, Optimum Clearance and Simulation. I. INTRODUCTION There are thousands of products manufactured with sheet metal parts. The first step in forming such a part involvescutting of the sheet into appropriate shapes by means of the physical process of shearing. A contoured part is cut between apunch and die in a press. Recent international market demands are that mechanical parts should be produced to net-shape ornear net-shape with improved mechanical properties, a smooth surface finish, good dimensional accuracy and materialsavings, depending on service conditions. In practice, manufacturing engineers are faced with the problem of determiningthe proper design of dies to cut metal sheets without causing any surface or internal defects at a lower manufacturing cost,depending on the material, the part geometry, and the process.1.1 The Blanking Process Blanking is a manufacturing operation as old as the technology itself. Its applications range from components ofvery light to heavy appliances and machineries [1].Blanking is defined as the cutting of a work piece between two diecomponents to a predetermined contour [2].During blanking, the part is subjected to complex solicitations such asdeformation, hardening and crack initiation and propagation. The theoretical modeling of such processes is very difficult dueto the complexity in describing the different stages of the whole shearing process starting with the elastic stage and endingwith the total separation of the sheet metal [3]. The behavior of the blank material during the blanking process can be divided into five stages. During the start ofthe process, the sheet is pushed into the die and the blank material is deformed, first elastically. The process continues andthe yield strength of the blank material is reached, first at the outer fibers and later at all the fibers in the zone between thepunch and the die. Normally, the material underneath the punch is subjected to thinning. The plastic deformation causesrounding of the edge of the blank. During this stage, or possibly as early as during the plastic deformation stage, damageinitiation followed by the nucleation and growth of cracks takes places. In most of the conventional blanking situations,ductile fracture occurs after shear deformation. This causes rough, dimpled rupture morphology on the fractured surface ofthe product. Finally, the work due to friction is dissipated when forcing (pushing) the slug through the die hole [4]. II. Literature Review The process of identifying process influencing parameters of blanking process includes an exhaustive literaturereview of the factors that have been suggested by various authors. Literature review was performed by collecting articlesfrom various journals, and various popular research related sites viz. Science Direct, IEEE, Emerald, Springer Link andvarious free articles from internet. Literature from journal papers and conference studied for various press tool worksparameters optimization are reviewed. S. K. Maiti, A. A. Ambekar, U. P. Singh, P.P. Date, K. Narasimhan, [1], they evaluate the influence of toolclearance, friction, sheet thickness, punch/die size and blanking layout on the sheet deformation for thin M. S. sheet. Thepunch load variation with tool travel and stress distribution in the sheet has been obtained. The results indicate that areduction in the tool clearance increases the blanking load. The blanking load increases with an increase in the coefficient offriction. These observations are very similar to the case of blanking of component of large size. Further, these effects arevery similar in the case of both single and double blanking. An inter blanking site distance of about twice the sheet thicknessis good to reduce the thinning of sheet at the intermediate regions between the two blanking sites. Ridha Hambli [3], presents industrial software called BLANKSOFT dedicated to sheet metal blanking processesoptimization. The code allows for the prediction of the geometry of the sheared profile, the mechanical state of the shearedzone, the burr height, the force–penetration curve, and the wear evolution of the punch versus the number of the blankingcycles. The approach is based on an original theoretical investigation formulated from plasticity theories. This program isdesigned by considering several factors, such as material and geometry of product as well as the wear state of the tool. Thenumerical results obtained by the proposed programs were compared with experimental ones to verify the validity of theproposed software. R. Hambli [5] , presents an experimental investigation into the blanking process was carried out using tools withfour different wear states (wear radius 0.01, 0.06, 0.012, 0.2 mm) and four different clearances (5%, 10%, 15%, 20%). Theaim was to study the effects of the interaction between the clearance, the wear state of the tool and the sheet metal thicknesson the evolution of the blanking force and the geometry of the sheared profile. He used designed of experiment method for www.ijmer.com 4547 | Page
2.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, Nov-Dec. 2012 pp-4547-4558 ISSN: 2249-6645model and analysis the relationships that describe process variations. This investigation shows that, in order to minimize theblanking force, the clearance should be set at 10%, however, to minimize the fracture angle and the fracture depth, it ispreferable to set the clearance at 5%. When the clearance is set at 10%, the process is slightly more robust to tool wear, as faras the blanking force response is concerned. Whether clearance should be set at 5% or 10% ultimately depends on thepriorities of the practitioners. F. Faura, A. Garcia, M. Estrems [6], they proposed a methodology to obtain optimum punch-die clearance valuesfor a given sheet material and thickness to be blanked, using the finite-element technique. To determine the optimumclearance, the diagonal angle and the angle of the direction of crack propagation for different clearances were calculated. Theinfluence of clearance on diagonal angle and angle of the direction of crack propagation, from which it is seen that as theclearance increases, diagonal angle increases proportionally while angle of the direction of crack propagation remainsnearly constant. At the point of intersection, the direction of crack propagation coincides with the diagonal line, and so thecracks emanating from the punch and die meet, resulting in a cleanly blanked surface. Hence, this value of clearance is takenas the optimum clearance. The optimum clearance for the values of the parameters used in this work is between 11 and 12%.It is observed that punch penetration increases as the c/t ratio increases. R. Hambli, S. Richir, P. Crubleau, B. Taravel [7] elaborates blanking process and structures of the blanked surfacesare influenced by both the tooling (clearance and tool geometry) and properties of the work piece material (blank thickness,mechanical properties, microstructure, etc.). Therefore, for a given material, the clearance and tool geometry are the mostimportant parameters. They use simulation of an ax symmetric blanking operation with ABAQUS- explicit software for agiven sheet material. A damage model of the Lemaitre type is used in order to describe crack initiation and propagation intothe sheet. They use four materials for testing with four different elongation (30%, 47%, 58%, and 65%).They show that theoptimum clearance decreases as the material elongation increases. The results of the proposed experimental investigationshow that there is no universal optimal clearance value. Whether clearance should be set at 5% or 10% ultimately dependson the priorities of the practitioners. Emad Al-Momani, Ibrahim Rawabdeh [8], Represents a model investigates the effect of potential parametersinfluencing the blanking process and their interactions. Finite Element Method (FEM) and Design of Experiments (DOE)approach are used in order to achieve the intended model objectives. They use Design of Experiments (DOE) technique byselecting the experimental levels for each selected factor, i.e. the clearance to be in five levels (5, 10, 15, 20, 25) % of thesheet metal thickness, blank holder force to be in two levels (0, 3000N) and sheet metal thickness to be in four levels (0.5,0.6, 0.7, 0.8)mm. Perform a factorial experimental design in order to take high-level interactions. Develop a Finite ElementModel (FEM) that represents the existing process in order to evaluate the quality of the inputs. Compare the two techniques(FEM and DOE) and analyze the results to get the proposed optimal set of parameters. Simulations are conducted oncommercial FEM software package ABAQUS/Explicit. in their article , they show that, in order to minimize the burrsheight, the clearance should be set at about 5 % with almost no blank holder force. Ridha Hambli [9], describes a methodology using the finite element method and neural network simulation in orderto predict the optimum punch–die clearance during sheet metal blanking processes. A damage model is used in order todescribe crack initiation and propagation into the sheet. The proposed approach combines predictive finite element andneural network modeling of the leading blanking parameters. Gang Fang*, Pan Zeng, Lulian Lou [10], in this paper, the punch–die clearance values for a given sheet materialand thickness are optimized, using the finite element technique and Cockcroft and Latham fracture criterion. In the study, theshearing mechanism was studied by simulating the blanking operation of an aluminum alloy 2024. The results of the presentpaper agree with the previous experimental results. III. FUNDAMENTALS OF THE THEORETICAL MODEL The errors on blanks are influenced by material, the tool shape, process variations and the machine. The form errorsrepresented in “Fig. (1)” are connected to the geometry of the sheared edge such as the roll-over depth, the fracture depth,the smooth-sheared depth, the burr formation and the fracture angle. Various experimental studies [17–23] showed that the mechanical and geometrical aspect of the sheared edgeduring the blanking operation for a given material are affected by some parameters like the blanking clearance, the wear stateof the tool and the thickness of the sheet. Figure. (1).Geometry of the sheared work piece www.ijmer.com 4548 | Page
3.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, Nov-Dec. 2012 pp-4547-4558 ISSN: 2249-66453.1. Deformation and rupture mechanism During sheet metal shearing operation, the part is subjected to complex solicitations such as deformation, hardeningand crack initiation and propagation. The theoretical modeling of such processes is very difficult due to the complexity ofdescribing the different stages of the whole shearing process starting from the elastic stage and ending to the total separationof the sheet metal” Fig ( 2)”. Figure. (2). Different stage of the blanking process. Accurate knowledge of the failure process is essential for the selection of a suitable damage model. In the case ofsheet blanking by shearing processes, numerous authors have studied the different physical mechanisms leading to the finalrupture, and proposed their own models. In their investigation dealing with a planar blanking process, Stegeman et al. [12] used a CCD camera records inorder to quantify the displacement of material points at the sheared surface “Fig.(3)”. One can observe the grid deformationin the Figure. (3). Grid deformation of material points during blanking process. Clearance zone of the tool. Recently, an analytical study and experimental tests [20, 21] showed that the physicalmechanisms leading to the complete failure of the sheet material can be described as follows. First, due to the penetration of the punch into the sheet, cracks initiate at the cutting edges „A‟ and „B‟ of the tools“Fig.(4)”. Secondly, the cracks propagate when and where Rice & Tracey fracture criterion value exceeds a critical value,and thus progressively cut the material fibers one after the other. The aforementioned rupture mechanism has been applied with success in a previous work [11] to numericallysimulate the whole blanking process until the final separation of the sheet. In this investigation, the mechanism model basedon the material cutting fibers has been applied to describe the deformation mechanism of the sheet metal during the shearingprocess. The main idea is to update incrementally the deformation mechanism in the clearance zone of the part for a givenpunch penetration increment. The equilibrium state of the part is then described using the concept of the continuummechanics theory. Figure. (4). Rupture of the sheet. A set of formulae taking into account the material characteristics of the sheet, the geometry of the operation and thewear state of the tool has been developed allowing for the prediction of the characteristic zone heights of the blanked partsuch the heights of the burr the roll-over, the sheared and the fractured zones. The punch penetration curve can also be plottedwhich allows for the computation of the maximum blanking force and the blanking energy. The equivalent plastic strainand equivalent stress of the sheared zone can be also predicted which permits the computation of the hardening state ofthe sheared zone. www.ijmer.com 4549 | Page
4.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, Nov-Dec. 2012 pp-4547-4558 ISSN: 2249-6645 IV. OPTIMUM CLEARANCE Various experimental studies [15,16,22,23,24,25,26] showed that the mechanical and geometricalaspect of the sheared edge during the blanking operation for a given material are affected by some parameters such as theblanking clearance, the wear state of the tool, and the thickness of the sheet. In blanking processes, the clearance is expressedin percentage of the sheet thickness and is defined by: 100 Dm − Dp % 𝑐= 2𝑡Where Dm, Dp and t are the die diameter, the punch diameter and the sheet thickness, respectively. In the case of blanking processes, one seeks to generate cracks at the sharp edges of the punch and thedie, then, through the choice of the parameters of cutting, attempt to make this crack propagate as soon as possible to obtaintotal rupture. In this investigation, it is assumed that the clearance is optimum when the direction of crackpropagation coincides with the line joining the points of crack initiation (A and B of “Fig.(5)” in the punch and die, givingcleanly blanked surfaces without secondary crack formation “Fig.(5)”. In this case, the total separation of the sheet isobtained for a lower value of punch penetration. If the cracks generated by the punch and die (A and B of “Fig.(5b)” do notcoincide, the formation of secondary cracks exists. Figure. (5). Secondary crack formation during blanking process. In order to obtain the optimum clearance value, the angle (θ) of the line joining the points of crackinitiation in the punch and die (diagonal angle) and the angle (β) of the direction of crack propagation must coincide“Fig.(6)”. This can be expressed by:θ= β The diagonal angle can be expressed by:θ=Arc tan(c/ t-up)Where up is the punch penetration corresponding to theFirst crack initiation within the sheet.4.1. Optimum Clearance Algorithm The optimum clearance value can be obtained by performing a series of numerical analyses in order to pursue aminimum cost function between the angle of the line joining the points of crack initiation in the punch and die θd (diagonalangle) and the angle of the direction of crack propagation (DCP) β “Figure (6)”. Figure. (6) Crack propagation angle and diagonal angle. www.ijmer.com 4550 | Page
5.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, Nov-Dec. 2012 pp-4547-4558 ISSN: 2249-6645During the optimization process a multi-variable objective function was chosen in the following form:Φ = βn – θdnβn is the direction of crack propagation angle at increment and θdn is the diagonal angle at increment n.The optimum clearance value can be obtained by performing a series of numerical analyses in order to pursue a minimumcost function between the angles θd and β.The global criteria of convergence are such that the numerical results must satisfy the following conditions:Abs (βn – θdn) ≤ Tol θdnTol. Is tolerance convergence value given by the user?Different simulations using different values of tolerance parameter showed that the final results are not sensitive to theselection of Tol.In this investigation, Tol. is taken equal to 10E-05.The iterative finite element program including the algorithm of the clearance optimization is schematically represented bythe following flow chart of “Figure (7)”.Incremental displacements are applied to the punch. At each increment, a fracture test is applied to each finite element of themesh. When the damage reaches its critical value at fracture Dc, the programs compute the angles βn and θdn. Figure. (7). Flow chart of calculation. V. FINITE ELEMENT METHOD (FEM) AND DESIGN OF EXPERIMENTS (DOE) Numerical methods provide a general tool to analyze arbitrary geometries and loading conditions. Among thenumerical methods, Finite Element Analysis (FEA) has been extensively used with success; however, this kind of analysisrequires the generation of a large set of data in order to obtain reasonably accurate results and consumes large investment inengineering time and computer resources [27]. FEM is a good choice for the analysis of sheet metal processes since it helpsin eliminating the need for time-consuming experiments to optimize the process parameters [1]. The FEM simulations areincreasingly used for investigating and optimizing the blanking processes. Many time-consuming experiments can bereplaced by computer simulations. Therefore, highly accurate results of sheet metal forming may be obtained by using theFEM simulation [28]. The finite element method gives an approximate solution with an accuracy that depends mainly on thetype of element and the fineness of the finite element mesh. In the manufacturing area, Design of Experiments (DOE) is found to be an efficient statistical technique that can beused for various experimental investigations. The design of experiments is one of the powerful tools used to investigatedeeply hidden causes of process variation [29]. It is a systematic, rigorous approach to engineering problem solving thatapplies principles and techniques at the data collection stage to ensure the generation of valid, defensible, and supportableconclusions. In the blanking process, experimental design is considered a powerful approach for product and process www.ijmer.com 4551 | Page
6.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, Nov-Dec. 2012 pp-4547-4558 ISSN: 2249-6645development, and for improving the yield and stability of an ongoing process. Hambli et al., [30] found that the design ofexperiments technique is an efficient and cost-effective way to model and analyze the relationships that describe processvariations. The sheet metal industry is highly interested in knowing if two identical products manufactured of two differentmaterials, can be blanked with a reasonable quality without the need to build two separate setups. This will increase theefficiency of the production processes and reduce the level of wasted materials, time, cost, and effort involved in theproduction stages. In addition, the industry needs a suitable model to overcome the long cycle time in developing a particularblanking process. This can be achieved by combining the Finite Element Method and Design of Experiments techniquesaiming at identifying opportunities to increase efficiency and productivity as well as eliminating waste and reducingproduction cost associated with the blanking process. The main objective of this paper is to construct a finite element modelto predict the shape of the cut side of a blanked product, and to investigate the effect of potential parameters influencing theblanking process and their interactions using the design of experiments approach in order to choose the process leadingparameters in an optimal way. VI. SIMULATION OF THE PROCESS6.1. FEM package The FEM program used to simulate the blanking process is ANSYS v. 5.1 [31], which is capable of solving thenon-linearity‟s of material behavior, large deformations, and contact between surfaces of different bodies. For the simulation described here, which is merely to determine the stress and strain of each node during theprocess, the use of specific codes devoted to simulating metal forming processes is not necessary.6.2. Model geometryThe following assumptions are made for the purposes of the present analysis: The process is simplified to a two-dimensional situation, under plane-strain conditions, since in a normal blanking operation the punch-die clearance is usually very small in relation to the blank diameter. The process is considered quasi-static, and hence the effects of strain rate are neglected. The sheet material is considered as a plastic object while the punch and die are defined as rigid bodies. Table I: summaries the geometric values used in the simulations. The tool wear geometry has been simulated by rounding off of the cutting edge (P-D radius). The friction contactbetween sheet and tool follows Coulomb‟s law: Tf = msnWhere Tf is friction shear stress, Sn is normal stress at interface, and m is the friction coefficient. “Fig. (8)”. Shows the finite element model. The increasing deformation in the simulation shows that the regionsbeyond a distance t from the shear zone undergo very much smaller deformation than that in the clearance zone. Moreover,the strains at the punch-die cutting edges reach the crack initiation value well before any significant deformation can takeplace in the region beyond t. Thus, the blanking operation is modeled by two rigid blocks, which are separated by a distancec and which move in opposite directions. Parameter Value Dimension Shearing gap c = (D-d)/2 M Clearance Cl = [(D-d)/2t] % 100 P-D radius r = 10- 4 M Friction µ= 0.05 coefficient Table I: Geometric parameter settingsD and d are punch and die diameters;t is thickness. www.ijmer.com 4552 | Page
7.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, Nov-Dec. 2012 pp-4547-4558 ISSN: 2249-6645 Figure. (8). Simulation model. In the blanking operation, deformation is concentrated along the very narrow shear band. The width of the shearband is a few microns. Thus, the number of elements used is critical for every simulation since a large number of elementsincreases the accuracy of the result, but also substantially increases the calculation time. Therefore, a very dense mesh wasdefined in the shearing band and relatively large elements for the remainder. It should also be mentioned that the CPU-timefor one simulation was about 10 h on an IBM RISC 6000 work station. VII. CASE STUDYDesign of Experiment Based Analysis for Sheet Metal Blanking Processes OptimizationR. HambliISTIA – LASQUO, Angers, France7.1 Material model In the present investigation, the optimum clearance was studied by simulating blanking of an AISI304 sheet with the specifications as in Table:2. It is assumed that the material is isotropic and that its yielding point follows the von Mises yield criterion. Abilinear representation of the stress – strain curve is used to model the behavior of the material, which is definedby two slopes: the elastic and the plastic slope. Figure. (9). Mesh in the shearing zone.7.2 Ductile fracture criterion (crack initiation criterion) Many experimental studies have been conducted to establish ductile fracture criteria in order to calculate theformability limits of different materials. Among the various fracture criteria proposed, it has been found that the criterionsuggested by Cockcroft and Latham [10] predicts the most reasonable fracture strain in metal forming operations. Thiscriterion states that fracture takes place when the following relation is satisfied: www.ijmer.com 4553 | Page
8.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, Nov-Dec. 2012 pp-4547-4558 ISSN: 2249-6645ε−ƒ σ∗ dε = 𝐶 σ0 Where σ* is the maximum principal tensile stress, ε-ƒ the fracture strain, and C the material constant. The effectivestress and effective strain are represented by σ¯ and ε¯, respectively.In the shearing operation, deformation is concentrated along the shear band the stress ratio (σ*/σ¯ ) is not expected to changealong the shear band. Parameter Value Dimension Thickness t=10- 3 M Yield Stress σy= 2.45· 108 Pa Elastic modules E= 1.225· 1011 Pa Tangent plastic Et= 1.586 · 109 Pa slope Table II: Material specifications Figure. (10). Electron microscopic observation on sheared blank (11% Clearance, 8 mm punch diameter). Therefore, Cockcroft and Latham‟s criterion may be approximated by ε-ƒ = C* at the shear band [7]. Consequently,it may be assumed that fracture takes place at a given effective strain. (During the blanking operation it is observed thatwhen the punch penetrates the sheet, the metal lying between the edges of the punch and the die (shearing gap) deformsseverely, and finally cracks are initiated. Crack initiation is a local phenomenon and in this methodology it is postulated thata crack is initiated at the point of the sheet whose effective strain first reaches the fracture strain of the work material. In thepresent investigation, the material constant, C* was obtained by measuring experimentally the punch penetration (∆) thatcauses a crack to begin, and computing numerically the maximum effective deformation for the punch penetration valuedetermined. According to the studies with worn tools presented in [1, 2], the crack does not emanate from the cutting edge butfrom the free surface. We considered that a crack starts in the punch-die flank at or just before the beginning of the radius ofthe cutting edges. The following values were obtained: ∆=7.5·10-4 m in the experimental “Fig. (10)”, and ε-ƒ = 3.88 in thenumericalSimulation.7.3 Optimum clearance In this investigation it is assumed that clearance is optimum when the direction of crack propagation coincides withthe line joining the points of crack initiation in the punch and die (diagonal line), giving cleanly blanked surfaces. Todetermine the optimum clearance, the diagonal angle (θ) and the angle of the direction of crack propagation (φ) for differentclearances were www.ijmer.com 4554 | Page
9.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, Nov-Dec. 2012 pp-4547-4558 ISSN: 2249-6645 C l(%) ∆ (%) φ (0 ) θ (0 ) 5 64 14.38 5.10 8 69.3 15.34 8.97 11 75 14.49 13.74 14 81.5 14.12 19.18 17 88.5 14.57 28.35 Table III: Punch penetration, diagonal angle and direction of crack Propagation for different clearances Calculated. It is postulated that cracks propagate perpendicularly to the maximum principal tensile stress [8]. In order to obtain the diagonal angle it is also assumed that the crack is initiated at or just before the radius of thecutting edges. The process to determine the optimum clearance can be observed in the flow chart represented in “Fig. (11)”.Successive displacements are imposed on the punch until any node (i ) fulfils the crack initiation criterion The values of theeffective strains, principal stress directions and punch penetration at crack initiation were obtained from the output of eachcomputer run. When the crack is initiated, the angle made by the diagonal with the y-axis was also calculated. Figure. (11). Flow chart to applied to determining the optimum clearance. Figure. (12). Simulated part edge (Cl=11%, ∆=75%).“Fig. (12)” shows the final edge of a simulation carried out with an 11% punch-die clearance and 75% punch penetration(percentages refer to the thickness of the sheet).7.4 Analysis of the results The values of the angles θ and φ were calculated for different clearances using the results of the finite-elementanalysis. These results are tabulated in Table 3, in which the punch penetration values (∆ as % of the thickness of the workmaterial) at crack initiation are also shown. “Fig. (13)” illustrates the influence of Cl on θ and φ, from which it is seen that asthe clearance increases, angle θ increases proportionally while angle φ remains nearly constant: the plots thus intersect. www.ijmer.com 4555 | Page
10.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, Nov-Dec. 2012 pp-4547-4558 ISSN: 2249-6645 Figure. (13). Variation of the diagonal angle and the direction of crack Propagation with the clearance. At the point of intersection, the direction of crack propagation coincides with the diagonal line, and so the cracksemanating from the punch and die meet, resulting in a cleanly blanked surface. Hence, this value of Cl is taken as theoptimum clearance. Figure. (14). Correlation between punch penetrations at crack initiation with Clearance. Figure. (15). Variation of angle of the direction perpendicular to the maximum principal tensile stress in node i, with punch penetration. The optimum clearance for the values of the parameters used in this work is between 11 and 12%, which is inagreement with previous experimental results and theoretical work [11, 12]. “Fig.(14)” illustrates the influence of clearanceon punch penetration at crack initiation, the results being similar to those of previous investigations [13]. It is observed thatpunch penetration increases as the c/t ratio increases. Consequently, with larger clearance, the severity of deformationdecreases, i.e. the material can deform more easily, so that greater punch penetration is necessary before cracks are initiated.“Fig.(15)” shows variations in the angle of the direction perpendicular to the maximum principal tensile stress in node i withincreasing punch penetration values, for different clearances. This figure shows how this angle reaches feasible values (interms of material fracture) for a range of punch penetration values similar to those observed experimentally at crackinitiation.7.5 Conclusions The methodology proposed makes it possible to predict optimum clearance using a general purpose FEM code for agiven sheet material and thickness to be blanked. In the absence of such an analytical method, a large number of experimentswould be required and their results would have to be analyzed carefully, for the optimum clearance to be calculated. Thehypothesis proposed in the present work regarding the point of crack initiation in the punch and die, which is used todetermine the values of C* and diagonal angle, closely reflects previous experimental results concerning optimum clearance. www.ijmer.com 4556 | Page
11.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, Nov-Dec. 2012 pp-4547-4558 ISSN: 2249-6645 REFERENCES[1] F.W. Timmerbil, Werkstatt. Maschin. 46 (1956) 58–66.[2] K. Buchmann, Werkstatt. Maschin. 53 (1963) 128–134.[3] F. Faura, J. Lo´ pez, C. Lu´ is, M.A. Sebastia´n, and Blanking of stainless steel: tool life equation model, in: T. Altan (Ed.), Advanced Technology of Plasticity, vol. II, Columbus, OH, 1996, pp. 655–663.[4] F. Faura, J. Lo´ pez, J. Sanes, Criterion for tool wears limitation on blanking 18-8 stainless steel strips, Rev. Metal. Madrid 33 (5) (1997) 304–310.[5] T. Altan, V. Vazquez, Numerical process simulation for tool and process design in bulk metal forming, Ann. CIRP 45 (1996) 599–615.[6] E. Taupin, J. Breitling, W.T. Wu, T. Altan, Material fracture and burr formation in blanking results of FEM simulations and comparison with experiments, J. Mater. Process. Technol. 59 (1996) 68–78.[7] S.H. Jeong, A study on shearing mechanism by FEM, MS Thesis, Seoul National University, Seoul, 1995.[8] D. Brokken, W.A.M. Brekelmans, F.P.T. Baaijens, Numerical analysis of the metal blanking process, in: T. Altan (Ed.), Advanced Technology of Plasticity, vol. II, Columbus, OH, 1996, pp. 665–668.[9] ANSYS User‟s Guide, ANSYS Inc., Houston, PA, 1995.[10] M.G. Cockcroft, D.J. Latham, A Simple Criterion of Fracture for Ductile Fracture of Metals, National Engineering Laboratory, Report No. 240, 1966.[11] T. Maeda, I. Aoki, The study on wear of blanking tool for 18-8 stainless steel and bainite hardened steel strips, J. Fac. Eng. Univ. Tokyo XXXII (3) (1974) 443–475.[12] A. Garcı´a, Estudio te´orico-experimental Del proceso de conformed de chapa por punzonado: modelos de prediccio´n Del juegode corte o´ptimo, Ph.D. Thesis, ETS Ingenieros Industriales, Univ. Murcia, Cartagena, 1997.[13] P.B. Popat, A. Ghosh, N.N. Kishore, Finite-element analysis of the blanking process, J. Mech. Work. Technol. 18 (1989) 269–282. VIII. CONCLUSION The experimental investigation of the sheet metal blanking process makes it possible to study the effects of processparameters such as the material type, the punch-die clearance, the thickness of the sheet and their interactions on thegeometry of the sheared edge especially the burrs height. Various methods are used in order to obtain a better understandingof the blanking manufacturing response. The investigation shows that, the blanking load increases with a reduction in the tool clearance in the case of bothsingle and double blanking. It is observed that the diagonal angle (θ) increases linearly according to the clearance, the crackpropagation angle (β) evolves nearly constant. One clear trend is that optimum clearance decreases as the material elongationincreases. There is no universal optimal clearance value in order to minimize the blanking force, the clearance should be set at10% and however, to minimize the fracture angle, the fracture depth and the burrs height; it is preferable to set theclearance at 5%. When the clearance is set at 10%, the process is slightly more robust to tool wear, as far as the blankingforce response is concerned. Whether clearance should be set at 5% or 10% ultimately depends on the priorities of thepractitioners. As a conclusion drawn from the proposed investigation, it is possible to optimize the sheet metalblanking process by a proper selection of the clearance. IX. FUTURE WORK Further investigation is needed to explore more parameters and operating conditions to develop a general model formore material types by using the combination of various techniques. A combination of techniques can be used in order toachieve a higher level of verification and to reduce the cost of the necessary experimental effort. It is recommended to experimentally perform the blanking process that combines the optimal set of parameters andmonitor its output quality. X. NOMENCLATURECl or c = Punch-Die Clearancet = Sheet ThicknessDm or D = Die DiameterDP or d = Punch Diameterθ = Diagonal AngleΒ or φ = Direction of Crack Propagation AngleUp = Punch PenetrationTol = Tolerance Convergence ValueTf = Friction Shear Stress,Sn = Normal Stress at Interface m = Friction Coefficient.r = Punch-Die Radiusµ = Friction Coefficient www.ijmer.com 4557 | Page
12.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, Nov-Dec. 2012 pp-4547-4558 ISSN: 2249-6645Σ* = the Maximum Principal Tensile Stress,Ε-ƒ = Fracture StrainC = Material Constant.σ¯ = Effective Stressε¯ = Effective StrainΣy = Yield StressE = Elastic ModulesET = Tangent Plastic Slope∆ = Punch Penetration REFERENCES[1] S. Maiti, A. Ambekar, U. Singh, P. Date, and K. Narasimhan, “Assessment of influence of some process parameters on sheet metal blanking”. Journal of Materials Processing Technology, Vol. 102, 2000, 249-256.[2] R. Hambli, “Finite element simulation of fine blanking process using a pressure-dependent damage model”. Journal of Materials Processing Technology, Vol. 116, 2001, 252-264.[3] R. Hambli, “BLANKSOFT: a code for sheet metal blanking processes optimization”. Journal of Materials Processing Technology, Vol. 141, 2003, 234-242.[4] W. Klingenberg, and Using, “Comparison of two analytical models of blanking and proposal of a new model”. International Journal of Machine Tools and Manufacture, Vol. 45, 2005, 519-527.[5] R. Hambli, (2002), “Design of Experiment Based Analysis for Sheet Metal Blanking Processes Optimization”. The International Journal of Advanced Manufacturing Technology, Vol.19, Page No.403-410.[6] F.F aura, A. Garcia and M. Estrems, (1998), “Finite element analysis of optimum clearance in the blanking process”. Journal of Materials Processing Technology, Vol.80-81, Page no.121-125.[7] R. Hambli, S. Richir, P. Crubleau, and B. Taravel, (2003), “Prediction of optimum clearance in sheet metal blanking processes”. International Journal of Advanced Manufacturing Technology, Vol. 22, page no. 20-25.[8] Emad Al-Momani, Ibrahim Rawabdeh, (Mar. 2008), “An Application of Finite Element Method and Design of Experiments in the Optimization of Sheet Metal Blanking Process” Jordan Journal of Mechanical and Industrial Engineering. Volume 2, Number 1, Pages 53 -63.[9] Ridha Hambli, (June 2005), “Optimization of blanking process using neural network simulation”, The Arabian Journal for Science and Engineering, Volume 30.[10] G. Fang, G., P. Zeng, and L. Lou, (2002), “Finite element simulation of the effect of clearance on the forming quality in the blanking process”. Journal of Materials Processing Technology Vol.122 page no. 249-254.[11] R. Hambli,A.Potiron, Finite element modeling o f sheet- metal blanking operations with experimental verification, J. Mater. Process.Technol. 102 (2000) 257–265.[12] Y.W. Stegeman, A.M. Goijaerts, D. Brokken, W.A.M. Brekelmans, L.E. Govaert, F.P.T. Baaijens, An experimental and numerical study of a planar blanking process, J. Mater. Process. Technol. 87(1–3, 15) (1999) 266–276.[13] A.G. Atkins, Surfaces produced by guillotining, Phil. Mag. 4 (1981) 627–641.[14] A.G. Atkins, Possible explanation for unexpected departures in hydrostatic tension–fracture strain relations, Metal Science, February 1981, pp. 81–83.[15] C.M. Choy, R. Balendra, Experimental analysis of parameters influencing sheared-edge profiles, in: Proceedings of the Fifth International Conference on Sheet Metal, University of Twente, The Netherlands, April 1–3, 1996, pp. 101–110.[16] T.M. Chang, Shearing of metal blanks, J. Inst. Met. 78 (1951) 393–414.[17] M. Cervenka, B. Bouchet, C. Gasc, Influence du mode de de´coupe sur le comportment en fatigue de toˆ les minces d‟aciers dual phase, Me´moires d‟e´tudes scientifiques Revue de me´tallurgie, March 1990, pp. 185–194.[18] Y. Kasuga, S. Tsutsumi, T. Mori, Investigation into shearing process of ductile sheet metals, Mem. Fac. Eng. Nagoya Univ., Japan, 1979, pp. 1–46.[19] S. Kalpakjian, Manufacturing Processes for Engineering Materials, 2nd ed., Addison-Wesley, Reading, MA, 1991.[20] R. Hambli, Numerical fracture prediction during sheet-metal blanking processes, Eng. Fract. Mech. 68 (3) (2000) 365–378.[21] R. Hambli, Etude expe´rimentale, nume´rique ET the´orique du decoupage des toˆ les en vue de l‟optimisation du proce´de´, Thesis Dissertation, ENSAM d‟Angers, 15 October 1996 (in French).[22] Atkins AG (1981) Surfaces produced by guillotining. Phil Mag 4:627–641[23] Kasuga Y,Tsutsumi S, Mori T (1979) Investigation into shearing process of ductile sheet metals. Mem Fac Eng Nagoya Univ, Japan, pp 1–46[24] Hambli R (1996) Etude experimental, numerique ET theorique du decoupage des toles en vue de l‟optimisation du procede (in French). Thesis dissertation, ENSAM, d‟Angers[25] Crisped MA (1991) Non linear ﬁnite element analysis of solids and structures, vol 1. Wiley, New York[26] BAQUS–HKS, Theory manual, Version 5.8[27] H. Andruet, “Special 2-D and 3-D Geometrically Nonlinear Finite Elements for Analysis of Adhesively Bonded Joints,” Unpublished Doctoral Dissertation, Virginia Polytechnic Institute, USA, 1998.[28] M. Samuel, “FEM simulations and experimental analysis of parameters of influence in the blanking process”. Journal of Materials Processing Technology, Vol. 84, 1998, 97-106.[29] Rawabdeh, H. Hilwa, and M. Abu Hammed, “Minimizing Necking Defects in Aluminum beverage Cans Using Experimental Design Techniques” .Dirasat, Engineering science, Vol. 30, No.1, 2003, 84-97.[30] R. Hambli, S. Richir, P. Crubleau, and B. Taravel, “Prediction of optimum clearance in sheet metal blanking processes”. International Journal of Advanced Manufacturing Technology, Vol. 22, 2003, 20-25.[31] ANSYS User‟s Guide, ANSYS Inc., Houston, PA, 1995. www.ijmer.com 4558 | Page
Be the first to comment